Magnetic States in Ensemble of Ferromagnetic Nanoparticles in Cu-Mn-Al Alloy
© Konoplyuk et al. 2016
Received: 30 November 2015
Accepted: 5 January 2016
Published: 14 January 2016
Two Cu-Mn-Al samples of different compositions were studied: one exhibiting martensitic transformation, another without structural transition. X-ray diffraction and magnetic measurements demonstrate that different magnetic behaviors of alloys originate from different concentrations and sizes of ferromagnetic nanoparticles, which appear after solid solution decomposition.
Estimation of magnetic moments of ferromagnetic nanoparticles from magnetization curves was performed using Langevin function and compared to those obtained from X-ray examination. Granular systems are known to show giant magnetoresistance. Therefore, magnetoresistance of Cu-Mn-Al melt-spun ribbons after different aging times was measured. The study has shown that increase in the concentration of Mn atoms and time of aging in Cu-Mn-Al alloy leads to an increase in the amount of precipitated phase appearing as ferromagnetic nanoparticles.
Magnetic phenomena related to spin-dependent electron scattering attract great attention as their study forms scientific basis for emerging technologies of ultrahigh-density recording and fabrication of magnetic sensors. Generally speaking, there are two main types of materials displaying spin-dependent scattering—multilayers and nanogranular systems . From the practical point of view, the most prospective is utilization of multilayers as they contain specific combination of layers tailored for concrete practical applications. Nanoscale granular systems including ensemble of ferromagnetic nanoparticles dispersed in nonmagnetic or antiferromagnetic matrix are of less practical interest, but they are interesting for fundamental science. The magnetic moments of these particles often referred to as “superspins” are dissipation centers for moving electrons. The magnetic field affects direction of “superspins” decreasing scattering of electrons and hence reducing electric resistance. This phenomenon called giant magnetoresistance, as well as other magnetic and transport properties of the nanogranular system, depends on a variety of parameters such as size, density, and magnetic moment of nanosized particles. They can couple each other by dipolar, exchange, or RKKY interactions . Collective behavior of nanoparticles can be modified to some extent by thermal treatment.
One of the alloys where formation of microstructure mentioned above occurs is Cu-Mn-Al one. In the Cu-Mn-Al system, there is a miscibility gap—the range of compositions wherein solid solution decomposition occurs. In this range according to , decomposition leads to appearance of ferromagnetic Cu2MnAl and nonmagnetic Cu3Al phases from solid solution below 623 K: the former has L21-ordered structure, the latter has DO3-ordered one. It was reported  that GMR in the Cu-Mn-Al system can achieve 15 %.
In other works, martensitic transformation occurring in this alloy was investigated. Results demonstrated that characteristic temperatures of the transformation decreased as Mn content was increased. In this system, Mn atoms play a significant role as only they possess magnetic moments providing ferromagnetism of Cu2MnAl compound. Therefore, changing concentration of Mn atoms, one can govern magnetic and transport properties of decomposed Cu-Mn-Al alloy. In this study, influence of Mn concentration and thermal treatment on the structure and properties of Cu-Mn-Al alloys was investigated.
The Cu-Mn-Al ribbons of two compositions were melt-spun: Sp1 (Cu-5 % Mn-23.4 % Al) and Sp2 (Cu-7 % Mn-26 % Al). Before crushing for melt spinning, the ingots were prepared by induction melting in argon atmosphere. Melt spinning was carried out by dropping the melt onto a copper wheel rotating with the velocity of 25 m/s. The fabricated ribbons were 100 μm thick. They were aged for 1, 2, 6, and 12 h to obtain different parameters of dispersed particles. Magnetization of ribbons was measured by the extraction technique using the commercial Physical Property Measurement System (PPMS) from Quantum Design. The samples for the magnetization measurements were prepared by crushing the Cu-Mn-Al ribbons into submillimeter parts and compacting them randomly in a gelatin capsule. Magnetoresistance was measured by four-terminal method along the direction of magnetic field and calculated as ratio ρ = (R(H) − R(0))/R(0) × 100 %, where H is the magnetic field and R(0) is the electric resistance of ribbon in zero field. X-ray diffraction patterns were obtained using CuKα radiation for Sp1 and CoKα for Sp2.
Results and Discussion
Melt spinning is the process in which melted alloy undergoes very fast cooling similar to quenching. It favors formation of a metastable state involving matrix and precipitated nanoparticles. For low content of Mn, decomposition along the Cu3Al-Cu2MnAl composition line yields formation of Cu2MnAl nanoparticles in Cu3Al matrix. X-ray diffraction is unable to determine the presence of precipitated particles if they are too small (less than several nanometers). But, aging promotes precipitation and growth of nanoparticles, and after this procedure, X-ray diffraction can detect them in structure. The Sp1 ribbon examined in this experiment was aged at 473 K for 2 h while the Sp2 one experienced the same treatment for 12 h.
Substituting values taken from Fig. 1b into (1) and (2), one can obtain 5 ± 1 nm as an average diameter of particle and 7 ± 1 nm as an average distance between the centers of particles. These values allow one to determine the concentration N and the volume fraction p of precipitated particles: N = 2.9 × 1018, p ~ 0.2. The estimated fraction p ~ 0.2 is consistent with that from the Cu3Al-Cu2MnAl phase diagram for particular alloy composition .
There are two basic states in the system of ferromagnetic nanoparticles in nonmagnetic matrix—superparamagnetic and superferromagnetic ones. Occurrence of the superferromagnetic state is attributed to interaction between nanoparticles leading to correlation between orientations of their magnetic moments. As it follows from estimations, the average distance between surfaces of inclusions (roughly 2 nm) excludes direct exchange interaction. In order to find out if other possible interactions are present in the ensemble of nanoparticles or its behavior is clearly superparamagnetic, magnetic measurements were carried out.
Blocking can originate from two reasons: individual blocking of magnetic moment of nanoparticle in the anisotropy field and the appearance of interaction between particles. Using expression T b = kV/25k B, where k is the magnetic anisotropy constant, V is the volume of particle, and k B is the Boltzmann constant, one can find that the blocking temperature due to anisotropy for Cu2MnAl particle of 5-nm diameter is less than 1 K. Hence, the first possible reason of “superspin” freezing can be excluded from consideration and, for all ribbons studied, the blocking temperature marks the onset of interparticle interaction on cooling.
According to , the atomic magnetic moment of Cu2MnAl is about 3 μ B per Mn atom and the unit cell measuring 0.59 × 0.59 × 0.59 nm3 incorporates four of them. This yields an average diameter of Cu2MnAl nanoparticles as 2.2 ± 0.5 and 5.5 ± 0.5 nm for the as-spun and aged Sp2 ribbons, respectively. Using saturation magnetization and calculated above parameters of the granular systems, one can easily estimate the concentration of nanoparticles and the interparticle distance: N = 1.35 × 1019, L = 4 nm for the as-spun alloy and N = 2.4 × 1018, L = 7.5 nm for the alloy aged for 6 h. The concentration and size of particles allowed to determine their volume fractions: 0.9 and 0.21, respectively. Lower value for the as-spun Sp2 ribbon implies that formation of phase precipitates after melt spinning is not completed. It is interesting to note that in spite of different ways of determination, the volume fractions of the Cu2MnAl phase in the sample aged for 6 h and that in the sample aged for 12 h are close to each other and correspond to the data from .
Results presented in this work demonstrate that magnetic and transport properties of the Cu-Mn-Al ribbons closely correlate with parameters of precipitated nanoparticles formed during solid solution decomposition. The ribbons of the Cu-5 % Mn-23.4 % Al composition do not show presence of coherent nanoparticles according to X-ray diffraction analysis even after aging for 2 h. It can be explained by a small size of them. This results in low magnetoresistance that does not exceed 0.1 %.
The ribbons of the Cu-7 % Mn-26 % Al composition demonstrate superparamagnetic behavior at room temperature irrespective of aging time. The estimations using magnetization curves fitted to Langevin function allowed for determination of the average particle size, the interparticle spacing, and the concentration of ferromagnetic nanoparticles. The volume fractions of Cu2MnAl nanoparticles in the Cu-7 % Mn-26 % Al ribbons demonstrated growth from 0.09 to 0.2 after the melt-spun ribbons were aged for 6 h. Aging also affected the magnetoresistance, increasing it with time during the first 3 h of the process. Magnetization measurements also revealed that freezing of magnetic moments at low temperatures characteristic of both the as-spun and the aged ribbons is most likely caused by the dipole-dipole interaction.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Shi J, Gider S, Babcock K, Awschalom DD (1996) Magnetic clusters in molecular beams, metals, and semiconductors. Science 271:937View ArticleGoogle Scholar
- Mydosh JA. Spin glasses: an experimental introduction. London: Taylor and Francis; 1993.Google Scholar
- Bouchard M, Thomas G (1975) Phase transition and modulated structures in ordered (Cu-Mn)3Al alloys. Acta Metall 23:1485View ArticleGoogle Scholar
- Yiping L, Murthy A, Hadjipanayis GC, Wan H (1996) Giant magnetoresistance in Cu-Mn-Al. Phys Rev B 54:3033View ArticleGoogle Scholar
- Kokorin VV. Martensitnye Prevrashchenia v Neodnorodnykh Tverdykh Rasvorakh (Martensitic transformations in inhomogeneous solid solutions). Kyiv: Naukova Dumka; 1987.Google Scholar
- Robinson J, McCormick P, Street R (1995) Structure and properties of Cu2MnAl synthesized by mechanical alloying. J Phys Condens Matt 7:4259View ArticleGoogle Scholar
- Zhang S (1992) Theory of giant magnetoresistance in magnetic granular films. Appl Phys Lett 61:1855View ArticleGoogle Scholar